International Journal of Corrosion
Volume 2016 (2016), Article ID 1343587, 7 pages
http://dx.doi.org/10.1155/2016/1343587

Research Article

A Probabilistic Physics of Failure Approach for Structure Corrosion Reliability Analysis

Chaoyang Xie1,2 and Hong-Zhong Huang¹

¹School of Mechatronics Engineering, University of Electronic Science and Technology of China, Chengdu 611731, China
²Institute of Systems Engineering, China Academy of Engineering Physics, Mianyang 621000, China

Received 14 January 2016; Revised 7 April 2016; Accepted 5 June 2016

Academic Editor: Ramana M. Pidaparti

Copyright © 2016 Chaoyang Xie and Hong-Zhong Huang. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Corrosion is recognized as one of the most important degradation mechanisms that affect the long-term reliability and integrity of metallic structures. Studying the structural reliability with pitting corrosion damage is useful for risk control and safety operation for the corroded structure. This paper proposed a structure corrosion reliability analysis approach based on the physics-based failure model of pitting corrosion, where the states of pitting growth, pit-to-crack, and cracking propagation are included in failure model. Then different probabilistic analysis methods such as Monte-Carlo Simulation (MCS), First-Order Reliability Method (FORM), Second-Order Reliability Method (SORM), and response surface method are employed to calculate the reliability. At last, an example is presented to demonstrate the capability of the proposed structural reliability model and calculating methods for structural corrosion failure analysis.

1. Introduction

Corrosion is recognized as one of the most important degradation mechanisms that affect the long-term reliability and integrity of metallic structures [1]. Corrosion can cause several kinds of defect on structure with the stress load and different corrosion environment, such as uniform corrosion, corrosion fatigue, pitting corrosion, and hydrogen embrittlement. As the increase of service time for metallic structure, the corrosion damage will grow, and the pit will change to a crack especially with static or circle loads. So the reliability and lifetime predictions of structure with pitting corrosion damage are significant for structure safety and risk mitigation.

The development of effective localized corrosion damage model is essential for reliability assessment. A simple empirical model was developed to describe the relationship between corrosion time and pitting depth based experimental data. In recent years, some stochastic method has been made in modeling pitting corrosion through Markov chains. Caleyo et al. used a nonhomogenous Markov process to model pit depth growth [2]. Valor et al. proposed a new stochastic model in which pitting initiation is modeled as a Weibull process [3]. Another type of corrosion damage model has been made based on electrochemical and mechanical process. Goswami and Hoeppner identified a seven-stage conceptual model for corrosion fatigue. The electrochemical effects in pit formation and the role of pitting in fatigue and corrosion fatigue crack nucleation behavior were considered in that model. Shi and Mahadevan represented a computational implementation approach based on the seven-stage conceptual model for corrosion fatigue life prediction [4]. Harlow and Wei proposed a three-stage probabilistic model including crack initiation, surface crack to grow into a through crack, and crack fracture. But all the models focus on structure with circle loads and the stress effect was not included in the pit growth phase. Stress corrosion crack is another important failure model for structure with static loads. Wu [5] proposed a probabilistic-mechanistic approach focused on modeling SCC propagation of Alloy 600 SG tubes with uncertainty. But the pit growth process was not contained in this model. A transition model for pitting to corrosion fatigue crack nucleation was first proposed by Kondo and further discussed by Harlow and Wei [6].

This paper proposed a physics-based failure model for structure with pitting corrosion damage. The mechanical stress effects for pitting growth are coupled in the integrated corrosion process. The three stages of pitting corrosion damage, pitting growth, pit-to-crack, and cracking propagation, are considered in the developed physics-based failure model. Then the time-dependent limit state function of corrosion structure is defined by fracture theory. The Monte-Carlo Simulation, FORM, and SORM are employed to calculate the reliability.

2. Reviews of Structure Reliability Analysis Method

2.1. MCS Method

Consider a performance model under the existence of uncertainties, where the system fails if . If the joint probability density function of random variables is , the statistical description of a probabilistic performance that fails is then completely characterized by the cumulative density function (CDF) as

In practice, the integration boundary and the high dimensionality make it difficult or even impossible to obtain an analytical solution to the probability integration in (11).

The MCS method is showed as follows [7, 8]:

where is the total number of simulations. is an indicator function. However the MCS method needs expensive computational cost.

2.2. FORM

The approximation methods are therefore used for reliability analysis in order to reduce the computational cost. FORM [9, 10] solves the probability integral by simplifying the performance function using the first-order Taylor series expansion at the Most Probable Point (MPP). The flowchart of the FORM for reliability analysis is shown in Figure 1. FORM involves three steps to approximate the integral [11, 12].

Figure 1: The flowchart of the FORM for reliability analysis.

Step 1. Transform original random variables in -space to standard normal random variables in -space, and the performance function is expressed as :

Step 2. Search for the Most Probable Point (MPP):

Step 3. After calculating, the reliability index β is obtained by an optimization problem. The probability in (1) is then computed analytically by the following equation:

2.3. SORM

In SORM [13–15], the performance function is approximated by the second-order Taylor series at MPP point. The approximation is given by

where is the Hessian matrix evaluated at the MPP; the gradient vector at MPP and the vector from MPP to the origin are parallel as

After a set of linear transformations, such as coordinate rotation and orthogonal diagonalization, the performance function is further simplified as

When is large enough, an asymptotic solution of the probability of failure can be then derived as

where denotes the th main curvature of the performance function . The approximation of the performance function in FORM and SORM is shown in Figure 2.

Figure 2: Comparison of FORM and SORM.

3. Physics of Failure Modeling for Pitting Corrosion

The degradation (damage) process for the crack development and propagation has been studied and modeled in many different ways [16]. In the proposed method, the pitting corrosion crack consists of four stages as shown in Figure 3.

Figure 3: Pitting corrosion growth process with stress.

The first stage in the corrosion damage process is pitting nucleation. It is related to the electrochemical process during corrosion, and the pit initial size and nucleation time depend on factors such as materials, corrosion environment, loads, and electrolytes. This process is very complex and the physics model of pit nucleation is not well understood yet. In this paper, we therefore assume the initial size of pit as a random variable. This distribution can be obtained by experimental data.

A simplified model for pit growth proposed by Harlow and Wei is used [6, 17]. The model assumes a pit of hemispherical shape growing at a constant volumetric rate in accordance with Faraday’s law from an initial radius size. The rate of pit growth is given as

where is the hemispherical pit volume, , is the pit size, is the molecular weight of the material, is the pitting current coefficient, is the valence, is Faraday’s constant, is the material density, is the activation energy, is the gas constant, and is the absolute temperature.

Based on the electrochemical theory, the electrical current on an electrode depends on the electrode potential. A general representation of the polarization of an electrode is described in the Butler-Volmer equation:

where is electrode current density, A/m², is exchange current density, A/m², is electrode potential, V, and is equilibrium potential, V. When the stress is applied on the metal materials with elastic deformation, the equilibrium potential will be varied according to Gutman’s theory [18, 19]:

where is the spherical part of macroscopic stress tensor excess pressure (Pa) and is the molar volume of the metal. The current density with the stress effects will be changed as

The coefficient- is used for depicting the variance of corrosion current with stress effects compared without stress situation.

In this paper, the effects of stress applied are considered based on (14); then the pit growing depth at the time can be changed to take into account the coupled effects of stress load and corrosion environment as

where is the pitting current, is the molar volume of the material, and is the bulk component of stress tensor. As the pit depth grows, the stress intensity factor at the pit tip will increase correspondingly and when it reaches a value beyond the threshold value of stress corrosion crack (SCC), the pit will transform into a crack and the SCC will thus occur. The criteria of a pit transforming into a crack can be obtained based on the thresholds of SCC and the fracture toughness as [6, 7]

where is the threshold of stress corrosion cracking and is the stress intensity factor for the surface of the pit. From the fracture mechanics theory, the critical size of a pit at the transition to a crack can be calculated as

where is the threshold stress intensity factor of SCC, which means the minimum stress required for SCC propagation, is the fracture toughness of the material, is the anodic polarization potential, α is the coefficient constant, is the yield stress, is shape factor, and is the stress concentration factor of the pit hole.

After the transition from a pit to a crack, the corrosion damage process will turn into the crack propagation stage. Unlike corrosion fatigue crack which is usually caused by the combination of cyclic load and a corrosive environment, the stress corrosion cracking is generally induced by a static tensile or torsional load to open and sustain the crack. The stress intensity factor at the crack propagation stage is generally a function of the total stress and the crack length. Similarly, the corrosion fatigue failure usually occurs once the stress intensity factor reaches a value beyond the threshold value . Following studies reported in the literature [12–14], in this study it is also assumed that the empirical model, as shown below, can be used for stress corrosion crack propagation, which is similar to the fatigue crack propagation modeled by Paris’ Law:

where and are the model constants of crack propagation. Note that the developed pit growth model takes into account the coupled effects of corrosion environment and the mechanical stresses at the pit growth stage of the corrosion damage process.

Following the terminology of structure reliability methods and stress-strength interference theory, corrosion failure can generally be defined as the stress intensity factor exceeding the fracture toughness based on fracture mechanics. Accordingly, with the assumptions that the corrosion pit of hemispherical shape grows at a constant volumetric rate, the corrosion current density with the stress effects will be changed as (3), and the pit will transform to crack when the stress effect dominates the corrosion pit growth, the corresponding time-dependent limit state function for corrosion reliability analysis can be written as

where is the shape parameter for the crake, is the static stress load, and is the pit depth in pitting growth stage or the crack size in crack propagation stage at a given time . Based on the time-dependent limit state function expressed in (10), denotes the safe state whereas represents the corrosion failure state.

4. Numerical Example

A case study is employed in this section to demonstrate the proposed physics of failure based corrosion model and reliability analysis approach. The case study structure is idealized as an infinite plate with a pitting corrosion defect while the pit corrosion occurs on the surface of the structure material, and the corrosive environment is assumed to be known. The structure material considered in this case study is the aluminum alloy, since it has been widely used in aerospace structures, energy engineering, and marine engineering applications. The uncertainties involved in material properties as well as the corrosion model parameters are considered and modeled with Gaussian random variables. The random and deterministic parameters used in this case study are listed in Tables 1 and 2, respectively [4, 6]. As shown in Table 1, seven different random variables are employed in this case study, as specified by the mean values and standard deviations, where the standard deviations for all random variables have been taken as 5% of the given mean values. To demonstrate the proposed corrosion model at the pit growth stage considering the coupled effects of corrosion environment and the mechanical stresses, the corrosion time has been assumed to begin right after the pit nucleation, and without losing the generosity the random pit nucleation has not been considered in this example.

Table 1: Random variables for case study.

Random variables
Unit
Mean
STD (mean%)

m

5%/10%

c/s

5%/10%

MPa/m²
35
5%/10%

MPa
470
5%/10%

Δσ
MPa
90
5%/10%

—

5%/10%

—
1.16
5%/10%

Table 2: Deterministic model parameters for the case study.

Variables
Value

2.6

1.15

0.12 V

2.6

27 g/mol

8.314 J/mol K

3

2.76 g/m³

96514 C/mol

50 KJ/mol

293 K

10 cm³/mol

Figure 4 provides 100 random realizations of the pit growth curve over time considering the random inputs as shown in Table 1. It is clear from the figure that the random inputs yield a large deviation for the pit growth curve over time and a few curves rising obviously after the pit transforms to crack propagation. Figure 5 shows that the value at the corrosion time equals 200 days. Note that the corrosion time does not include the pit nucleation time.

Figure 4: Pit depth growth curve with different corrosion time.

Figure 5: value distribution at days.

The structure reliability of pitting corrosion damage is calculated using MCS and FORM. The MCS is used with a large number of samples () as the benchmark solution to check the accuracy of the FORM method. With the random variables shown in Table 1, the corrosion reliability analysis is then carried out with different corrosion times using two different approaches as mentioned earlier and the analysis results are summarized in Tables 3 and 4. The comparison of the reliability estimations and the absolute percentage errors obtained using the FORM and SORM compared with the MCS results are also shown in Figures 6 and 7. It is clear from the figures that the reliability estimation error for the FORM tends to increase with longer corrosion time, mainly due to the linearization of the limit state the FORM used. Besides the accuracy performance, the efficiencies of corrosion reliability analysis using the FORM, SORM, and MCS are also compared, as the results shown in Table 4, in which the number of sample points being evaluated for the limit state function is employed as the accuracy measure. As shown in the table, the FORM generally requires less sample points to be evaluated to conduct reliability analysis, compared with the MCS method. The results also show that the FORM is more efficient than SORM, but its calculation accuracy is lower than SORM. Moreover, due to the gradient-based searching process employed by the FORM to find the MPP, the gradient information must be provided, where in this study the finite difference method has been employed for the FORM to provide the required information. As the gradient-based method is used for MPP search, the searching process may not converge to the true MPP efficiently in some scenarios, as shown in the table for corrosion time of 250 days and 300 days in which the total numbers of sample evaluations for both have reached the upper limit of 800.

Table 3: The reliability results with different corrosion time.

Corrosion time (days)
Reliability

MCS
FORM
FORM error (%)
SORM
SORM error (%)

250
0.99815
0.99868
0.05310
0.99834
0.01903

300
0.99113
0.99496
0.38643
0.99302
0.02

350
0.97036
0.98297
1.29952
0.97843
0.083

400
0.93395
0.95372
2.11682
0.94532
1.2174

450
0.88074
0.90589
2.85555
0.89740
1.8916

500
0.81476
0.84112
3.23531
0.83059
1.943

Table 4: Comparison of computational efficiencies for FORM and SORM.

Corrosion time (days)
250
300
350
400
450
500

Number of functions evaluated (FORM)
800
800
136
232
288
128

Number of functions evaluated (SORM)
800
800
347
489
548
571

Figure 6: Reliability analysis results at different corrosion times.

Figure 7: The computational error of FORM and SORM.

5. Conclusion and Future Work

The pitting corrosion growth model considering the coupled effects of stress and corrosion environment is proposed based on mechanical theory. And the time-dependent limit state function is discussed for stress corrosion crack failure based on the corrosion growth model. MCS and FORM are used for reliability assessment approaches. The example shows that the model is useful for structure reliability analysis, but the model parameters need verification by more experimental data. Apply this mechanical model for structure corrosion failure prognostics. Integrate the Bayesian inference method for parameter estimation.

Competing Interests

The authors declare that they have no competing interests.

Acknowledgments

This work was supported by the Foundation of China Academy Engineering Physics (CAEP) under Grant no. 2013B0203028 and the Technology Foundation Project under Grant no. 2013ZK1.2.

References

R. E. Melchers, “The effect of corrosion on the structural reliability of steel offshore structures,” Corrosion Science, vol. 47, no. 10, pp. 2391–2410, 2005.

F. Caleyo, J. C. Velázquez, A. Valor, and J. M. Hallen, “Markov chain modelling of pitting corrosion in underground pipelines,” Corrosion Science, vol. 51, no. 9, pp. 2197–2207, 2009.

A. Valor, F. Caleyo, L. Alfonso, D. Rivas, and J. M. Hallen, “Stochastic modeling of pitting corrosion: a new model for initiation and growth of multiple corrosion pits,” Corrosion Science, vol. 49, no. 2, pp. 559–579, 2007.

P. Shi and S. Mahadevan, “Damage tolerance approach for probabilistic pitting corrosion fatigue life prediction,” Engineering Fracture Mechanics, vol. 68, no. 13, pp. 1493–1507, 2001.

G. Wu, A probabilistic-mechanistic approach to modeling stress corrosion cracking propagation in alloy 600 components with applications [M.S. thesis], University of Maryland, College Park, Md, USA, 2011.

D. G. Harlow and R. P. Wei, “A probability model for the growth of corrosion pits in aluminum alloys induced by constituent particles,” Engineering Fracture Mechanics, vol. 59, no. 3, pp. 305–325, 1998.

A. Haldar and S. Mahadevan, Probability, Reliability and Statistical Methods in Engineering Design, John Wiley & Sons, New York, NY, USA, 2000.

H. J. Pradlwarter and G. I. Schuëller, “Local domain Monte Carlo simulation,” Structural Safety, vol. 32, no. 5, pp. 275–280, 2010.

G. J. Li, Z. Z. Lu, and C. C. Zhou, “Discussion on: local domain Monte Carlo simulation: H. J. Pradlwarter and G. I. Schueller, Structural Safety, 32 (2010) 275–280,” Structural Safety, vol. 40, pp. 78–80, 2012.

M. Di Sciuva and D. Lomario, “A comparison between Monte Carlo and FORMs in calculating the reliability of a composite structure,” Composite Structures, vol. 59, no. 1, pp. 155–162, 2003.

Y.-G. Zhao and T. Ono, “A general procedure for first/second-order reliability method (FORM/SORM),” Structural Safety, vol. 21, no. 2, pp. 95–112, 1999.

A. Der Kiureghian, “The geometry of random vibrations and solutions by FORM and SORM,” Probabilistic Engineering Mechanics, vol. 15, no. 1, pp. 81–90, 2000.

J. Lim, B. Lee, and I. Lee, “Second-order reliability method-based inverse reliability analysis using hessian update for accurate and efficient reliability-based design optimization,” International Journal for Numerical Methods in Engineering, vol. 100, no. 10, pp. 773–792, 2014.

M. Hohenbichler and R. Rackwitz, “Improvement of second-order reliability estimates by importance sampling,” Journal of Engineering Mechanics, vol. 114, no. 12, pp. 2195–2199, 1989.

J. Zhang and X. Du, “A second-order reliability method with first-order efficiency,” Journal of Mechanical Design, vol. 132, no. 10, Article ID 101006, 2010.

M. C. Alseyabi, Structuring a probabilistic model for reliability evaluation of piping subject to corrosion-fatigue degradation [Ph.D. thesis], University of Maryland, College Park, Md, USA, 2009.

C. Xie, P. Wang, Z. Wang, and H. Huang, “Probability of corrosion failure analysis using an adaptive sampling approach,” in Proceedings of the IEEE Conference on Prognostics and Health Management (PHM '15), pp. 1–8, Austin, Tex, USA, June 2015.

E. M. Gutman, Mechanochmistry of Solid Surfaces, World Scientific Publications, Singapore, 1994.

X. G. Jiang, W. Y. Zhu, and J. M. Xiao, “Fractal analysis of orientation effect on KIC and KISCC,” Engineering Fracture Mechanics, vol. 51, no. 5, pp. 805–808, 1995.